you would be aware about the different types of special concrete being used in india.All these types of concrete are being produced by ultratech concrete, for more details visit
you would be aware about the different types of special concrete being used in india.All these types of concrete are being produced by ultratech concrete, for more details visit www.ultratechconcrete.com/concrete_types.html
• Concrete is most vital material in modern
• In addition to normal concrete, other
varieties in use are, high strength and high
performance concrete, self compacting,
light weight, high density, fibre reinforced,
polymer, coloured concrete etc.
• The making of concrete is an art as well as
• Special types of concrete are those with out-of-theordinary properties or those produced by unusual
techniques. Concrete is by definition a composite
material consisting essentially of a binding medium and
aggregate particles, and it can take many forms.
• These concretes do have advantages as well as
1.High Volume Fly Ash Concrete.
• Is used to replace a portion of the portland cement used in the mix.
• According to IS: 456 – 2000 replacement of OPC by Fly-ash up to
35% as binding material is permitted.
• HVFAC is a concrete where excess of 35%of fly-ash is used as
• Use of fly ash is because of many factors such as
a) Abundance of fly ash i.e. 110million tons of fly ash is produced in India
b) Fly ashes from major TPP are of very high quality i.e. quality of fly ash.
c) Economic factor i.e. Cost of fly ash with in 200 km from a TPP is as low
as 10% to 20% of the cost of cement.
d) Environmental factors i.e. reduction in CO2 emission.
Strength relation between control concrete and fly
Permeability relation between control
and fly ash concrete.
2.Silica fume concrete
• Very fine non-crystalline silica produced in electric arc furnaces as a
• Highly reactive pozzolan used to improve mortar and concrete.
• Silica fume in concrete produces two types of effect viz.
• Physical effect
• Chemical effect
• The transition zone is a thin layer between the bulk hydrated cement
paste and the aggregate particles in concrete. This zone is the
weakest component in concrete, and it is also the most permeable
area. Silica fume plays a significant role in the transition zone
through both its physical and chemical effects.
• The presence of any type of very small
particles will improve concrete
properties. This effect is termed either
“particle packing” or “micro filling”.
• physical mechanisms do play a
significant role, particularly at early
Silica fume is simply a very effective
pozzolanic means a siliceous or siliceous and
aluminous material, which in itself possess
little or no cementious value but will, in finely
divided form and in the presence of moisture
, chemically react with calcium hydroxide at
ordinary temperatures to form compounds
possessing cementious properties.
3. GGBS, Slag based concrete
• By-product of the iron manufacturing industry, replacement of
Portland cement with GGBS will lead to significant reduction of
carbon dioxide gas emission.
• GGBS powder is almost white in colour in the dry state Fresh
GGBS concrete may show mottled green or bluish-green areas on
the surface mainly due to the presence of a small amount of
• GGBS concrete requires longer setting times than Portland cement
concrete, probably due to the smooth and glassy particle forms of
GGBS. If the temperature is 23oC or replacement level of portland
cement by GGBS is less than 30% , the setting times will not
significantly be affected.
• when GGBS replacement level is less than 40%, bleeding is
generally unaffected. At higher replacement levels, bleeding rates
may be higher.
• GGBS concrete has lower early strengths because the rate of initial
reaction of GGBS is slower than that of Portland cement. GGBS is
therefore generally grounded to a finer state than Portland cement i.e. from
around 4000 cm2/g to 6000 cm2/g resulting in significant increase in 28day strength.
• It was also reported that the early strengths (up to 28 days) of concrete
mixes (with 25%, 35%, 50%, and 60% GGBS replacements) were lower
than that of Portland cement concrete mixes. By 56 days, the strength of
50% and 60% GGBS mixes exceeded that of the Portland cement mix, and
by one year all GGBS mixes were stronger than the Portland cement mixes.
• Due to its longer setting time, it can be transported to distant places but
care should be taken while casting because there are chances that bleeding
may take place.
4. Ternary blend concrete
• Ternary concrete mixtures include three different cementitious
materials i.e. combinations of portland cement, slag cement, and a
third cementitious material. The third component is often fly ash,
but silica fume is also common.
• Other material in combination with portland and slag cement, such
as rice husk ash are not currently in common usage.
• Slag cement has been used in ternary mixtures for decades.
1. High strength
2. Low permeability
3. Corrosion resistance
4. Sulphate resistance
5. ASR resistance
6. Elimination of thermal cracking
Ternary mixtures can be used and have been used in
virtually any concrete application
1. General construction (residential, commercial, industrial)
3. High performance concrete
4. Precast concrete
5. Masonry and masonry units
6. Mass concrete
The optimum mixture proportions for ternary blends, as with other concrete,
will be dependent on the final use of the concrete, construction requirements
and seasonal considerations. As with other concrete, cold weather will affect
the early strength gain and mixture proportions may need to be adjusted to
assure job-site performance. In low W/CM applications such as paving,
mixtures with 15percent fly ash and 30% slag cement component have been
Fly ash, a powder resembling
cement, has been used in
concrete since the 1930s.
Ground granulated blast
Silica fume powder
5.Light weight concrete
• Structural lightweight concrete is similar to normal weight concrete except
that it has a lower density.
• Made with lightweight aggregates.
Air-dry density in the range of 1350 to 1850 kg/m3
28-day compressive strength in excess of 17 Mpa.
Structural lightweight concrete is used primarily to reduce the dead-load
weight in concrete members, such as floors in high-rise buildings.
• Structural Lightweight Aggregates:
Rotary kiln expanded clays, shales, and slates
Sintering grate expanded shales and slates
Pelletized or extruded fly ash
• Compressive Strength:
The compressive strength of structural lightweight
concrete is usually related to the cement content at a given slump and air content,
rather than to a water-to-cement ratio. This is due to the difficulty in determining
how much of the total mix water is absorbed into the aggregate and thus not
available for reaction with the cement.
Due to lower aggregate density, structural lightweight concrete does not slump
as much as normal-weight concrete with the same workability.
A lightweight air-entrained mixture with a slump of 50 to 75 mm (2 to 3 in.) can
be placed under conditions that would require a slump of 75 to 125 mm (3 to 5
With higher slumps, the large aggregate particles tend to float to the surface,
making finishing difficult.
Entrained Air in light-weight concrete
• Entrained Air:
As with normal-weight concrete, entrained air in structural lightweight concrete ensures
resistance to freezing and thawing and to deicer applications.
It also improves workability, reduces bleeding and segregation, and may compensate for
minor grading deficiencies in the aggregate.
Air contents are generally between 5% and 8%, depending on the maximum size of coarse
aggregate (paste content) used and the exposure conditions.
Placing, Finishing, and Curing
1. Structural lightweight concrete is generally easier to handle and place than
2. A slump of 50 to 100 mm (2 to 4 in.) produces the best results for
3. If pumped concrete is being considered, the specified suppliers and
contractor should all be consulted about performing a field trial using the
pump and mixture planned for the project.
4. Adjustments to the mixture maybe necessary.
5. pumping pressure causes the aggregate to absorb more water, thus
reducing the slump and increasing the density of the concrete.
Polymer concrete is part of group of concretes that
use polymers to supplement or replace cement as a
binder. The types include polymer-impregnated
concrete, polymer concrete, and polymer-Portlandcement concrete.
• In polymer concrete, thermosetting resins are used as the principal polymer
component due to their high thermal stability and resistance to a wide variety of
• Polymer concrete is also composed of aggregates that include silica, quartz,
granite, limestone, and other high quality material.
• Polymer concrete may be used for new construction or repairing of old concrete.
The low permeability and corrosive resistance of polymer concrete allows it to be
used in swimming pools, sewer structure applications, drainage channels,
electrolytic cells for base metal recovery, and other structures that contain liquids
or corrosive chemicals.
• It is especially suited to the construction and rehabilitation of manholes due to
their ability to withstand toxic and corrosive sewer gases and bacteria commonly
found in sewer systems.
• It can also be used as a replacement for asphalt pavement, for higher durability
and higher strength.
• Polymer concrete has historically not been widely adopted due to the high costs
and difficulty associated with traditional manufacturing techniques.
Advantages & Disadvantages
Rapid curing at ambient temperatures
High tensile, flexural, and compressive
Good adhesion to most surfaces
Good long-term durability with respect to
freeze and thaw cycles
Low permeability to water and aggressive
Good chemical resistance
Good resistance against corrosion
Lighter weight (only somewhat less dense
than traditional concrete, depending on the
resin content of the mix)
May be vibrated to fill voids in forms
10. Allows use of regular form-release agents (in
1. Product hard to manipulate with
conventional tools such as drills and
presses due to its strength and density.
Recommend getting pre-modified
product from the manufacturer
2. Small boxes are more costly when
compared to its precast counterpart
however pre cast concretes induction
of stacking or steel covers quickly
bridge the gap.
7.Self compacting concrete
• Self-compacting concrete (SCC) is an innovative concrete that does not require
vibration for placing and compaction. It is able to flow under its own
weight, completely filling formwork and achieving full compaction, even in the
presence of congested reinforcement.
• The hardened concrete is dense, homogeneous and has the same engineering
properties and durability as traditional vibrated concrete.
• Very close to the Kolhapur there is project of steel industry, sand used for the
formation of mould when the moulds are opened the waste sand is dumped for
the filling the low lying areas while doing this the agriculture areas is converted
into barren area. Because there is no space for the waste other than the land
filling. similar case is in case of aluminium industry where red mud is
concluded to be waste, which contains lot amount of bauxite and that is why
red mud is also dump in the nearby areas here it is causing big threat for the
society and it is disturbing the eco system of the environment. So it is the need
to use this particular otherwise waste material for the constructive in such
fashion in the case of concrete so that concrete which became cost effective as
well as eco-friendly.
Powder type of self-compacting concrete: This is proportioned to give the required
self-compactability by reducing the water-powder ratio and provide adequate segregation
Viscosity agent type self-compacting concrete: This type is proportioned to provide
self-compaction by the use of viscosity modifying admixture to provide segregation
Combination type self-compacting concrete: This type is proportioned so as to obtain
self-compactability mainly by reducing the water powder ratio.
• Fresh SCC Properties:
1. Filling ability (excellent deformability)
2. Passing ability (ability to pass reinforcement without blocking)
3. High resistance to segregation.
• It has been observed that the compressive strength of
selfcompacting concrete produced with the combination of
admixtures goes on increasing up to 2% addition of red mud.
• After 2% addition of red mud, the compressive strength starts
decreasing, i.e. the compressive strength of self-compacting
concrete produced is maximum when 2% red mud is added.
• The percentage increase in the compressive strength at 2%
addition of red mud is +9.11 .
• Coloured concrete can be produced by using coloured aggregates or by
adding colour pigments (ASTM C 979) or both.
• If surfaces are to be washed with acid, a delay of approximately two weeks
after casting is necessary.
• Coloured aggregates may be natural rock such as quartz, marble, and
granite, or they may be ceramic materials.
• synthetic pigments generally give more uniform results.
• The amount of colour pigments added to a concrete mixture should not be
more than 10% of the mass of the cement.
• .For example, a dose of pigment equal to 1.5% by mass of cement may
produce a pleasing pastel colour, but 7% may be needed to produce a deep
colour. Use of white portland cement with a pigment will produce
cleaner, brighter colours and is recommended in preference to gray
cement, except for black or dark gray colours.
9. Fibre reinforced concrete:
• Fibre reinforced concrete (FRC) may be defined as a composite materials
made with Portland cement, aggregate, and incorporating discrete
• The role of randomly distributes discontinuous fibres is to bridge across
the cracks that develop provides some post- cracking “ductility”.
• The real contribution of the fibres is to increase the toughness of the
concrete under any type of loading.
• The fibre reinforcement may be used in the form of three – dimensionally
randomly distributed fibres throughout the structural member when the
added advantages of the fibre to shear resistance and crack control can
be further utilised.
• Tensile Strength:
Fibres aligned in the direction of the tensile stress may bring about very large increases
in direct tensile strength, as high as 1.33% for 5% of smooth, straight steel fibres.
Thus, adding fibres merely to increase the direct tensile strength is probably worthwhile.
However, as in compression, steel fibres do lead to major increases in the post cracking
behaviour or toughness of the composites.
• Application of SFRC:
The most common applications are
2. tunnel linings
3. pavements and slabs
5. shotcrete also containing silica fume, airport pavements, bridge deck slab repairs
The fibres themselves are, unfortunately, relatively expensive; a 1% steel fibre addition
will approximately double the rate.
• Pervious (porous or no-fines) concrete contains a narrowly graded coarse
aggregate, little to no fine aggregate, and insufficient cement paste to fill
voids in the coarse aggregate.
• Low water-cement ratio, low-slump concrete resembling popcorn held
together by cement paste.
• Produces a concrete with a high volume of voids (20% to 35%) and a high
permeability that allows water to flow through it easily.
• Pervious concrete is used in hydraulic structures as drainage media, and in
parking lots, pavements, and airport local groundwater supply by allowing
water to penetrate the concrete to the ground below.
• Pervious concretes have also been used in tennis courts and greenhouses.
• The compressive strength of different mixes can range from 3.5 to 27.5
• Drainage rates commonly range from 100 to 900 lit.per minute per square
11. Water-proof concrete:
Top Proof waterproof concrete contains two
specially formulated admixtures. The first reduces
the water/cement ratio, increasing the density of
the mix and minimising the size of the pores. The
second fills the remaining pores ensuring a
completely watertight finish. This means there is
no need for external membranes, reducing cost and
Waterproof concrete benefits:
Waterproof concrete applications:
1. No need for external
membranes, reducing cost and
2. Water resistant, quality-assured
2. Underground car parks
3. Electrical and other plant rooms
4. Swimming pools
3. Less susceptible to cracking
5. Aquariums and aquatic centres
4. No minimum order size
6. Waterside buildings
5. 100% recyclable
12. Mass concrete:
• “An large volume of cast-in-place concrete with dimensions large enough
to require that measures be taken to cope with the generation of heat and
attendant volume change to minimize cracking.”
• Mass concrete includes not only low-cement-content concrete used in dams
and other massive structures but also moderate to high cement content
concrete in structural members of bridges and buildings.
As the interior concrete increases in temperature and expands, the surface
concrete may be cooling and contracting.
• The width and depth of cracks depends upon the temperature
differential, physical properties of the concrete, and the reinforcing steel.